ASTM-C1332 › Standard Practice for Measurement of Ultrasonic Attenuation Coefficients of Advanced Ceramics by Pulse-Echo Contact Technique
Show Complete Document History
The following bibliographic material is provided to assist you with your purchasing decision:
Changes from the previous issue
A redline edition is available for this document, with all changes visible. Ask Document Center Inc. for more information.
1.1 This practice describes a procedure for measurement of ultrasonic attenuation coefficients for advanced structural ceramic materials. The procedure is based on a broadband buffered piezoelectric probe used in the pulse-echo contact mode and emitting either longitudinal or shear waves. The primary objective of this practice is materials characterization.
1.2 The procedure requires coupling an ultrasonic probe to the surface of a plate-like sample and the recovery of successive front surface and back surface echoes (refer to ). Power spectra of the echoes are used to calculate the attenuation spectrum (attenuation coefficient as a function of ultrasonic frequency) for the sample material. The transducer bandwidth and spectral response are selected to cover a range of frequencies and corresponding wavelengths that interact with microstructural features of interest in solid test samples.
1.3 The purpose of this practice is to establish fundamental procedures for measurement of ultrasonic attenuation coefficients. These measurements should distinguish and quantify microstructural differences among solid samples and therefore help establish a reference database for comparing materials and calibrating ultrasonic attenuation measurement equipment.
1.4 This practice applies to monolithic ceramics and also polycrystalline metals. This practice may be applied to whisker reinforced ceramics, particulate toughened ceramics, and ceramic composites provided that similar constraints on sample size, shape, and finish are met as described herein for monolithic ceramics.
1.5 This practice sets forth the constraints on sample size, shape, and finish that will assure valid attenuation coefficient measurements. This practice also describes the instrumentation, methods, and data processing procedures for accomplishing the measurements.
1.6 This practice is not recommended for highly attenuating materials such as very thick, very porous, rough-surfaced monolithics or composites. This practice is not recommended for highly nonuniform, heterogeneous, cracked, defective, or otherwise flaw-ridden samples that are unrepresentative of the nature or inherent characteristics of the material under examination.
1.7 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety, health, and environmental practices and determine the applicability of regulatory limitations prior to use.
1.8 This international standard was developed in accordance with internationally recognized principles on standardization established in the Decision on Principles for the Development of International Standards, Guides and Recommendations issued by the World Trade Organization Technical Barriers to Trade (TBT) Committee.
attenuation coefficient; attenuation spectrum; material microstructure; materials characterization; monolithic ceramics; nondestructive evaluation; polycrystalline metals; pulse-echo technique; ultrasonic attenuation; ultrasonics;; ICS Number Code 81.060.30 (Advanced ceramics)
To find similar documents by ASTM Volume:
To find similar documents by classification:
19.100 (Non-destructive testing Including testing equipment: industrial apparatus for X-ray and gamma radiography, penetrant flaw detectors, etc. Non-destructive testing of welded joints, see 25.160.40 Industrial radiographic films, see 37.040.25 Non-destructive testing of metals, see 77.040.20)
This document comes with our free Notification Service, good for the life of the document.
This document is available in either Paper or PDF format.
Revision with Title Change
Feb. 1, 2018